LMucko/crystallography-open-database huggingface dataset:
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 901 C, held for 16h, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005957
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 901 C, held for
 16h, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0473
_cell_length_b                   8.0473
_cell_length_c                   8.0473
_cell_volume                     521.135
_database_code_amcsd             0007539
_exptl_crystal_density_diffrn    4.503
_exptl_crystal_thermal_history   'quenched from 901 C, held for 16h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005957
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 950 C, held for 16h, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005958
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 950 C, held for
 16h, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0481
_cell_length_b                   8.0481
_cell_length_c                   8.0481
_cell_volume                     521.291
_database_code_amcsd             0007540
_exptl_crystal_density_diffrn    4.502
_exptl_crystal_thermal_history   'quenched from 950 C, held for 16h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005958
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1000 C, held for 1h, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005959
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1000 C, held for
 1h, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0488
_cell_length_b                   8.0488
_cell_length_c                   8.0488
_cell_volume                     521.427
_database_code_amcsd             0007541
_exptl_crystal_density_diffrn    4.501
_exptl_crystal_thermal_history   'quenched from 1000 C, held for 1h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005959
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1050 C, held for 1h, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005960
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1050 C, held for
 1h, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0497
_cell_length_b                   8.0497
_cell_length_c                   8.0497
_cell_volume                     521.602
_database_code_amcsd             0007542
_exptl_crystal_density_diffrn    4.499
_exptl_crystal_thermal_history   'quenched from 1050 C, held for 1h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005960
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1100 C, held for 35m, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005961
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1100 C, held for
 35m, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0504
_cell_length_b                   8.0504
_cell_length_c                   8.0504
_cell_volume                     521.738
_database_code_amcsd             0007543
_exptl_crystal_density_diffrn    4.498
_exptl_crystal_thermal_history   'quenched from 1100 C, held for 35m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005961
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1150 C, held for 5m, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005962
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1150 C, held for
 5m, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0511
_cell_length_b                   8.0511
_cell_length_c                   8.0511
_cell_volume                     521.874
_database_code_amcsd             0007544
_exptl_crystal_density_diffrn    4.497
_exptl_crystal_thermal_history   'quenched from 1150 C, held for 5m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005962
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1200 C, held for 10m, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005963
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1200 C, held for
 10m, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0517
_cell_length_b                   8.0517
_cell_length_c                   8.0517
_cell_volume                     521.991
_database_code_amcsd             0007545
_exptl_crystal_density_diffrn    4.496
_exptl_crystal_thermal_history   'quenched from 1200 C, held for 10m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005963
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1250 C, held for 10m, Bayerisheches Geoinstitut (Mo), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005964
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1250 C, held for
 10m, Bayerisheches Geoinstitut (Mo), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0522
_cell_length_b                   8.0522
_cell_length_c                   8.0522
_cell_volume                     522.088
_database_code_amcsd             0007546
_exptl_crystal_density_diffrn    4.495
_exptl_crystal_thermal_history   'quenched from 1250 C, held for 10m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005964
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 700 C, held for 43d, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005965
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 700 C, held for 43d, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0452
_cell_length_b                   8.0452
_cell_length_c                   8.0452
_cell_volume                     520.728
_database_code_amcsd             0007547
_exptl_crystal_density_diffrn    4.507
_exptl_crystal_thermal_history   'quenched from 700 C, held for 43d'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005965
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 750 C, held for 80h, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005966
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 750 C, held for 80h, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0460
_cell_length_b                   8.0460
_cell_length_c                   8.0460
_cell_volume                     520.883
_database_code_amcsd             0007548
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'quenched from 750 C, held for 80h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005966
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 750 C, held for 43h, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005967
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 750 C, held for 43h, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0460
_cell_length_b                   8.0460
_cell_length_c                   8.0460
_cell_volume                     520.883
_database_code_amcsd             0007549
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'quenched from 750 C, held for 43h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005967
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 800 C, held for 11d, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005968
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 800 C, held for 11d, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0460
_cell_length_b                   8.0460
_cell_length_c                   8.0460
_cell_volume                     520.883
_database_code_amcsd             0007550
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'quenched from 800 C, held for 11d'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005968
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 850 C, held for 49h, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005969
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 850 C, held for 49h, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0460
_cell_length_b                   8.0460
_cell_length_c                   8.0460
_cell_volume                     520.883
_database_code_amcsd             0007551
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'quenched from 850 C, held for 49h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005969
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 901 C, held for 16h, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005970
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 901 C, held for 16h, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0473
_cell_length_b                   8.0473
_cell_length_c                   8.0473
_cell_volume                     521.135
_database_code_amcsd             0007552
_exptl_crystal_density_diffrn    4.503
_exptl_crystal_thermal_history   'quenched from 901 C, held for 16h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005970
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 950 C, held for 16h, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005971
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 950 C, held for 16h, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0481
_cell_length_b                   8.0481
_cell_length_c                   8.0481
_cell_volume                     521.291
_database_code_amcsd             0007553
_exptl_crystal_density_diffrn    4.502
_exptl_crystal_thermal_history   'quenched from 950 C, held for 16h'
_cod_duplicate_entry             9005958
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005971
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1000 C, held for 1h, UCLA (Cu), Model 1
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005972
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 1000 C, held for 1h, UCLA (Cu), Model 1
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0488
_cell_length_b                   8.0488
_cell_length_c                   8.0488
_cell_volume                     521.427
_database_code_amcsd             0007554
_exptl_crystal_density_diffrn    4.501
_exptl_crystal_thermal_history   'quenched from 1000 C, held for 1h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005972